|Year : 2021 | Volume
| Issue : 1 | Page : 6-12
|Influence of the surface energy of different brands of polymethyl methacrylate on the adherence of Candida albicans: An in vitro study
Betty Cabanillas1, Adrián Mallma-Medina2, Marieta Petkova-Gueorguieva3, Daniel Alvitez-Temoche1, Román Mendoza1, Frank Mayta-Tovalino4
1 Academic Department, Faculty of Dentistry, Universidad Nacional Federico Villarreal, Lima, Peru
2 Academic Department, Faculty of Dentistry, Universidad Nacional Federico Villarreal, Lima, Peru; Academic Department of Basic Sciences, Faculty of Dentistry, Universidad Nacional Mayor de San Marcos, Lima, Peru
3 Academic Department of Basic Sciences, Faculty of Dentistry, Universidad Nacional Mayor de San Marcos, Lima, Peru
4 Academic Department of Rehabilitative Stomatology, Faculty of Dentistry, Universidad Nacional Mayor de San Marcos, Lima, Peru; Postgraduate Department, Faculty of Health Sciences, Universidad Cientifica del Sur, Lima, Peru
|Date of Submission||14-Jun-2020|
|Date of Decision||21-Jun-2020|
|Date of Acceptance||09-Jul-2020|
|Date of Web Publication||30-Jan-2021|
Dr. Frank Mayta-Tovalino
Avenue Paseo de la República 5544, Miraflores 15074, Lima.
Source of Support: None, Conflict of Interest: None
| Abstract|| |
Objective: The objective of this study was to evaluate the influence of the surface energy of different brands of polymethyl methacrylate (PMMA) on the adherence of Candida albicans ATCC 10231 in an in vitro study. Materials and Methods: The study had an in vitro, longitudinal, and comparative experimental design. The following groups were made: (1) Vitacryl versus controls (water, dimethyl sulfoxide, glycerol, diethylene glycol, and formamide); (2) Triplex versus the same controls; (3) Vitacryl versus Triplex (surface energy); and (4) Vitacryl versus Triplex (adhesion per cell/field). Adhesion was measured in the area of each field magnified 10 × 10, and with an increase in magnification to 40 × 10, very dense colonies of 0.152 mm2 were observed. Results: The surface energy of Vitacryl and Triplex was 40.3 ± 0.3 and 39.5 ± 0.3N/m, respectively, showing statistically significant differences (P < 0.001). On the contrary, in relation to the adhesion per cell/field of C. albicans, Vitacryl presented 15.7 ± 1.1, whereas Triplex had 16.7 ± 2.3, with no significant differences (P = 0.058). Conclusion: In relation to the adhesion per cell/field of C. albicans, there was no evidence of significant differences between Vitacryl and Triplex.
Keywords: Adherence, Candida albicans, polymethyl methacrylate, surface energy
|How to cite this article:|
Cabanillas B, Mallma-Medina A, Petkova-Gueorguieva M, Alvitez-Temoche D, Mendoza R, Mayta-Tovalino F. Influence of the surface energy of different brands of polymethyl methacrylate on the adherence of Candida albicans: An in vitro study. J Int Soc Prevent Communit Dent 2021;11:6-12
|How to cite this URL:|
Cabanillas B, Mallma-Medina A, Petkova-Gueorguieva M, Alvitez-Temoche D, Mendoza R, Mayta-Tovalino F. Influence of the surface energy of different brands of polymethyl methacrylate on the adherence of Candida albicans: An in vitro study. J Int Soc Prevent Communit Dent [serial online] 2021 [cited 2021 Mar 5];11:6-12. Available from: https://www.jispcd.org/text.asp?2021/11/1/6/308386
| Introduction|| |
Biomaterials are biological materials used to replace some lost living tissue. A biomaterial is a pharmacologically inert and biocompatible component in a living system.,, These components restore the functions of the tissues of the lost body, and therefore, it is important to understand the relationships between the functions and properties of these biological materials.,
Along history, various materials have been used in the manufacture of denture bases, including wood, bone, ivory, metals, and numerous polymers such as polymethyl methacrylate (PMMA), polystyrene, polyamide, epoxy resin, polycarbonate, and vulcanite. The selection of the different specific materials is based on availability, cost, physical properties, aesthetic qualities, and handling characteristics. From different materials used, PMMA shows the best properties, and as a result, it currently dominates the field of denture bases.,,
One of the physical properties of denture bases that has been studied is surface energy, which directly influences the amount of microorganisms, such as bacteria and fungi, which the surface of a biomaterial can retain. Surface energy can determine the presence or absence of adherence of microorganisms. It is composed of the sum of the intermolecular forces that are on the surface of a body, that is, it corresponds to the degree of attraction that the surface of one material exerts on another. For example, when a body has a high surface energy, it has a high tendency to attract itself, while the adhesive has a low possibility of surface tension.,, In the search for new substances and/or biomaterials, it is also important to control microorganisms such as Candida albicans in the oral cavity.,,,
Therefore, the objective of this study was to assess the influence of the surface energy of different brands of PMMA on the adherence of C. albicans ATCC 10231 in an in vitro study.
| Materials and Methods|| |
The study had an in vitro, longitudinal, and comparative experimental design, and was carried out in the Microbiology Laboratory of the Faculty of Dentistry of the Universidad Nacional Federico Villarreal, Lima, Peru. The independent variable was the surface energy of the acrylic resins, and the dependent variable was the adherence of C. albicans ATCC 10231. The sample size was obtained by the means comparison formula using Stata 15 software (College Station, TX, USA). Each brand of PMMA had an n = 18.
The following four groups were formed:
- Group 1: PMMA Vitacryl versus controls (water, glycerol, formamide, diethylene glycol, and dimethyl sulfoxide) [Figure 1]
- Group 2: PMMA Triplex versus controls (water, glycerol, formamide, diethylene glycol, and dimethyl sulfoxide)
- Group 3: PMMA Vitacryl versus PMMA Triplex (surface energy) [Figure 2]A and [B]
- Group 4: PMMA Vitacryl versus PMMA Triplex (adhesion per cell/field)
|Figure 2: (A) Contact angle between glycerol and a sample of Vitacryl. (B) Contact angle between formamide and a Triplex sample|
Click here to view
Polymethyl methacrylate preparation
PMMA was prepared from a wax master model with dimensions of (15 × 10 × 1 mm). Each type of acrylic was processed according to the manufacturer’s specifications. The procedures known as packaging, polymerization, muffling, and demuffling were applied, for which the same type of plaster was used, and the entire procedure was carried out after calibration. The brands of acrylic resins were: Vitacryl (A. Tarrillo Barba, Lima, Peru) and Triplex (Ivoclar Vivadent, Ellwangen, Germany). Eighteen samples were prepared for each type of acrylic. The samples were examined using a magnifying glass (×50), and those with superficial defects or pores were discarded, for both brands of acrylics.,,
C. albicans strain ATCC 10231 was reactivated in 0.5mL of Sabouraud dextrose broth and incubated for 24 h at 37°C. On completion of the growth period, it was verified that C. albicans was in the yeast phase, cultured on Sabouraud dextrose agar. The separation of the yeasts from the culture broth was carried out by centrifugation at 1200rpm for 10min, and then washed with 10 cc of phosphate-buffered saline (PBS). After centrifugation of the tubes with the cultures, the broth was removed and the pellet was left, and 0.5mL of PBS was added to this. After three washings with PBS, an optical density of 0.5 was achieved according to the McFarland scale standard, which corresponds to 1.5 × 108 cells/mL.,
Incubation of polymethyl methacrylate samples
The samples of both brands were kept in distilled water for 17 days, renewing the water daily, to achieve saturation. One polymer sample per tube was placed, and 2mL of yeast suspension was added. After verifying that the sample was completely covered, the samples were incubated for 2 h at 37°C. At the end of the incubation period, the samples were removed from the incubator and rinsed twice with 25mL of sterile PBS for 1min by gentle manual shaking. This process allows the elimination of the yeasts not adhered to the polymer samples.,,
Evaluation of microbial adhesion
Once the samples were dry, the yeasts were stained with acridine orange at a concentration of 0.003%. The samples were placed in Petri dish More Detailses adding 15 drops of the acridine orange solution to the surface and staining for 10min, and then allowed to dry. Nine fields were counted on each sample, the areas selected for the count were evenly distributed on the surface of the sample. The area of each field was magnified 10 × 10, and with an increase in the magnification to 40 × 10, very dense colonies of 0.152 mm2 were observed, [Figure 3]A and [B].
|Figure 3: (A) Candida albicans cells in the Vitacryl sample, stained with 0.003% acridine orange, viewed under a fluorescence microscope (×10). (B) C. albicans cells in the Triplex sample, stained with 0.003% acridine orange, seen under a fluorescence microscope (×10)|
Click here to view
Descriptive analysis used measures of central tendency and dispersion (mean, standard deviation, minimum, and maximum). Normality was determined using the Shapiro–Wilk test. Subsequently, the Student’s t test was performed because of the homogeneity of the data. Finally, to determine correlations among numerical variables, linear regression was used. All the analyses were evaluated with a significance level of P < 0.05. All the data were analyzed using Stata 15 software.
| Results|| |
The angle between the surface and the Vitacryl was 48.1° ± 0.5° in the group, whereas the diethylene glycol and dimethyl sulfoxide control groups showed the lowest angulation with 34.6° ± 0.3° and 14.6° ± 0.5°, respectively. On the contrary, the distribution in the PMMA (Vitacryl) group was not normal in the chemical substances Vitacryl, water, and formamide (P < 0.05) [Graph 1] [Table 1].
|Graph 1: Comparison of angle between the surface of polymethyl methacrylate Vitacryl and Triplex versus different chemical experimental substances|
Click here to view
|Table 1: Angle evaluation between the surface of PMMA Vitacryl and Triplex versus different chemical substances|
Click here to view
In the PMMA (Triplex) group, the angle between the surface and the Triplex was 47.3° ± 0.2°. As in the previous group, the control chemicals, diethylene glycol and dimethyl sulfoxide, had the lowest angulation with 33° ± 0.6° and 15.0° ± 0.4°, respectively [Graph 1] [Table 1].
The surface energy of PMMA (Vitacryl) and PMMA (Triplex) was 40.3 ± 0.3 and 39.5 ± 0.3N/m, respectively, showing statistically significant differences (P < 0.001).
In relation to the adhesion per cell/field of C. albicans, PMMA (Vitacryl) presented 15.7 ± 1.1, whereas PMMA (Triplex) had 16.7 ± 2.3, with these differences being nonsignificant (P = 0.058) [Table 2].
|Table 2: In vitro evaluation of the surface energy and adhesion per cell/field of Candida albicans according to the polymethyl methacrylate type Vitacryl and Triplex|
Click here to view
Finally, linear regression analysis showed that in the PMMA group (Vitacryl), for each unit of surface energy in N/m, the adhesion per cell/field of C. albicans can be expected to increase by a statistically significant mean of 0.112 (P < 0.001) [Graph 2]. In contrast, in the PMMA group (Triplex), the P = 0.329 suggested that changes in the predictors are not associated with changes in response [Table 3].
|Graph 2: Regression scatter plot and linear prediction of surface energy and adhesion per cell/field of C. albicans according to the polymethyl methacrylate type Vitacryl and Triplex|
Click here to view
|Table 3: Linearregression of surface energy and adhesion per cell/field of Candida albicans according to the type of polymethyl methacrylate Vitacryl and Triplex|
Click here to view
| Discussion|| |
Biomaterials are artificial substances (polymers, ceramics, and metals, among others), used in living organisms to modify or replace some tissue, organ, or function. It is desirable to have a biomaterial with surfaces that are not adherent to bacterial or fungal cells, as these colonies are responsible for the pathogenesis of an organism. Knowledge of the characteristics that influence the adherence of these colonies must be taken into account in the choice and processing of biomaterials. One of these characteristics is the surface energy of microorganisms and biomaterials, as this is directly proportional to the retention of cells present between one and the other. In this sense, it is necessary to know which type of acrylic resin (PMMA) has the least adherence in relation to C. albicans.,,, The essential characteristic that all biomaterials must fulfill is biocompatibility, which is understood as the quality of not inducing toxic or harmful effects to the biological systems in which they operate, and performing an appropriate host response in a specific situation.
The characteristics of the immune system are such that when a foreign body is introduced into the body, it tends to reject or even attack it. Biocompatibility has a compatibility index, which indicates whether or not this material is suitable for use in a living being, taking into account its application.,,,,
The association of C. albicans with prosthetic stomatitis is important but is not a determining factor for the appearance of disease. Studies determining the microorganisms present in the plaque associated with prosthetic stomatitis have shown that depending on the degree of disease, the presence of C. albicans is more or less frequent. The main causes of prosthetic stomatitis are trauma, infection, and allergy to the components of the prosthesis. However, studies such as that by Budtz-Jörgensen explained that the appearance of the disease was determined by multiple factors, one determining factor being the systemic condition of the individual. The adhesion of C. albicans to the surface of PMMA is very complex due to the large number of factors involved. For this reason, some in vitro studies carried out to date often report contradictory results. For example, this is the case with respect to the role of saliva, although it is accepted that saliva plays a protective role in relation to prosthetic stomatitis.
In a study on the relationship between the amount of saliva and the C. albicans count in individuals with prosthetic stomatitis, Navazesh et al. found no significant relationship between these two variables. This study was of note as it evaluated a variable not usually determined in most in vitro studies such as the present. This variable is the adhesion between fungi and the prosthesis. Indeed, some studies have described greater adhesion of C. albicans in PMMA samples treated with saliva.
The diversity of methods used in the literature makes it difficult to compare results even when using the same system, as there is no established protocol, and each author or work group uses the C. albicans strain that seems most suitable for their study. The same occurs with respect to yeast concentrations, incubation times, and temperature, as well as the procedure to eliminate nonadherent yeasts or the staining method. Another problem related to methodology is the choice of the appropriate staining system for the yeast count per field. Using a self-curing type of transparent PMMA, polymer samples thin enough to allow yeast counting by transmission light microscopy and the use of a dye can be obtained.,,
In this study, the relationship between the surface energy of PMMA and the adhesion of C. albicans from Triplex and Vitacryl was analyzed, showing that for each unit of surface energy in N/m, the adhesion per cell/C. albicans field significantly increased by a mean of 0.112 (P < 0.001). This high correlation has also been found in some studies, when comparing the surface energy of two different Candida (albicans and tropicalis) with their adherence to thermoset resins.,,
It should be noted that when viewing of the control samples (C. albicans in an acridine orange–stained petri dish) was performed under the fluorescence microscope, C. albicans was observed in the form of yeast, whereas, on the contrary, in the experimental samples (C. albicans in acrylic plate stained with acridine orange), cells in the form of pseudohyphae were observed. None of the previously mentioned studies have reported this finding. C. albicans shows great adhesive capacity to not only host cells but also to inert materials such as acrylic resins, largely due to the chemical and structural characteristics of the cell walls, aided by the characteristics provided by the medium.
The main limitation of this study was that as there was no established protocol for the process of sample preparation, incubation, staining, and colony counting, the processes were performed based on experimental methodology. Although PMMA sample making measurements are based on the dimensions of a conventional test tube and on the manufacturer’s specifications, there is no standard for polishing. The polishing of conventional total or partial prostheses is carried out differently for the external and the internal faces. The internal part must be the most adapted to the palate mucosa, and thus, the polishing criterion should be respected for studies on acrylic resin samples in subsequent in vitro studies. Another limitation was that when the acrylic resin samples are submerged in the medium during the incubation procedure, they should be suspended by some device, as, if they are allowed to submerge completely in the broth, the plate will sink to the bottom of the container, which will allow only one side of the sample to be in contact with the culture broth, whereas the other side will be in direct contact with the container.
According to the results of this study, it is recommended that the incubation process should use a shaker that provides sufficient movement to ensure that the cells are suspended and in uniform contact with the acrylic resin sample. Regarding staining, the location and use of liquid acridine orange was one of the greatest difficulties encountered when performing the present investigation. As this is not essential for the staining of C. albicans colonies, it is recommended to use another type of dye. In addition, acridine orange stains use viable and nonviable cells, which can be used in subsequent investigations related to that already described, such as cell counting.
The results of this research have a direct impact on the stomatognathic system. One of the most frequent alterations is the loss of dental pieces producing partial or total edentulism, leading to the need for oral rehabilitation treatments using partial or complete prostheses. In both cases, the base material for these prostheses is thermosetting acrylic resin. The lack of adequate clinical and technical management and the failure of patients to comply with medical instructions, as well as a possibly suppressed immune system, can lead to the development of opportunistic diseases such as subprosthetic stomatitis that is directly related to the colonization of different pathogens including C. albicans. In addition to the aforementioned factors, there are acrylic resin factors derived from each manufacturing company, which can act directly on a greater or lesser retention of bacterial plaque. Although in this study, samples were not obtained from individuals with prosthetic stomatitis, the results and the microphotographs of the cultures may be useful for future comparison with the studies by the aforementioned authors.
| Conclusion|| |
In conclusion, the PMMA group (Vitacryl) showed that for each surface energy unit in N/m, the adhesion per cell/field of C. albicans can be expected to significantly increase by a mean of 0.112. In contrast, in the PMMA group (Triplex), the P value suggested that changes in the predictor are not associated with changes in response. Significant differences were found between the surface energy of PMMA (Vitacryl) and PMMA (Triplex). Finally, in relation to the adhesion per cell/field of C. albicans, no significant differences were found between PMMA (Vitacryl) and PMMA (Triplex).
We wish to thank Universidad Nacional Federico Villarreal.
Financial support and sponsorship
Conflicts of interest
There are no conflicts of interest.
Study conception was by BC and AMM; data collection by BC and AMM; data acquisition and analysis by FMT, DAT, and RM; data interpretation by RM, FMT, and MPG; and manuscript writing by FMT, MPG, AMM, and DAT.
Ethical policy and institutional review board statement
This project was exempted from ethical approval as it was an experimental in vitro study.
Patient consent statement
Data availability statement
The data that support the study results are available from the corresponding author (Dr. Frank Mayta-Tovalino, e-mail: [email protected]) on request.
| References|| |
Serrano-Granger C, Cerero-Lapiedra R, Campo-Trapero J, Del Río-Highsmith J In vitro
study of the adherence of Candida albicans
to acrylic resins: Relationship to surface energy. Int J Prosthodont 2005;18:392-8.
Park SE, Periathamby AR, Loza JC Effect of surface-charged poly(methyl methacrylate) on the adhesion of Candida albicans
. J Prosthodont 2003;12:249-54.
Yodmongkol S, Chantarachindawong R, Thaweboon S, Thaweboon B, Amornsakchai T, Srikhirin T The effects of silane-SiO2 nanocomposite films on Candida albicans
adhesion and the surface and physical properties of acrylic resin denture base material. J Prosthet Dent 2014;112:1530-8.
Straioto FG, Alves R, Filho AP, Del Bel Cury AA Polytetrafluoroethylene added to acrylic resin: Surface properties and Candida albicans
adherence. Am J Dent 2010;23:201-4.
Lee JH, El-Fiqi A, Jo JK, Kim DA, Kim SC, Jun SK, et al
. Development of long-term antimicrobial poly(methyl methacrylate) by incorporating mesoporous silica nanocarriers. Dent Mater 2016;32:1564-74.
Moura JS, da Silva WJ, Pereira T, Del Bel Cury AA, Rodrigues Garcia RC Influence of acrylic resin polymerization methods and saliva on the adherence of four Candida
species. J Prosthet Dent 2006;96:205-11.
Breguła L, Trzeciak H, Nolewajka-Lasak I [The study of adhesion of Candida albicans
to the selected acrylic resins]. Med Dosw Mikrobiol 2006;58:67-71.
Zhou L, Tong Z, Wu G, Feng Z, Bai S, Dong Y, et al
. Parylene coating hinders Candida albicans
adhesion to silicone elastomers and denture bases resin. Arch Oral Biol 2010;55:401-9.
Poma-Castillo L, Espinoza-Poma M, Mauricio F, Mauricio-Vilchez C, Alvítez-Temoche D, Mayta-Tovalino F Antifungal activity of ethanol-extracted Bixa orellana
(L) (Achiote) on Candida albicans
, at six different concentrations. J Contemp Dent Pract 2019;20:1159-63.
Gómez C, Salcedo-Moncada D, Ayala G, Watanabe R, Pineda M, Alvítez-Temoche D, et al
. Antimicrobial efficacy of calcium and sodium hypochlorite at different concentrations on a biofilm of Enterococcus faecalis
and Candida albicans
: An in vitro
comparative study. J Contemp Dent Pract 2020;21:178-82.
Calderon A, Salas J, Dapello G, Gamboa E, Rosas J, Chávez J, et al
. Assessment of antibacterial and antifungal properties and in vivo
cytotoxicity of Peruvian Passiflora mollisima
. J Contemp Dent Pract 2019;20:145-51.
Kang SH, Lee HJ, Hong SH, Kim KH, Kwon TY Influence of surface characteristics on the adhesion of Candida albicans
to various denture lining materials. Acta Odontol Scand 2013;71:241-8.
Panagoda GJ, Ellepola AN, Samaranayake LP Adhesion to denture acrylic surfaces and relative cell-surface hydrophobicity of Candida parapsilosis
and Candida albicans
. APMIS 1998;106:736-42.
Budtz-Jörgensen E The significance of Candida albicans
in denture stomatitis. Scand J Dent Res 1974;82:15190.
Samaranayake LP Nutritional factors and oral candidosis. J Oral Pathol 1986;15:615.
Navazesh M, Wood GJ, Brightman VJ Relationship between salivary flow rates and Candida albicans
counts. Oral Surg Oral Med Oral Pathol Oral Radiol Endod 1995;80:284-8.
Edgerton M, Levine MJ Characterization of acquired denture pellicle from healthy and stomatitis patients. J Prosthet Dent 1992;68:683-91.
Azuma A, Akiba N, Minakuchi S Hydrophilic surface modification of acrylic denture base material by silica coating and its influence on Candida albicans
adherence. J Med Dent Sci 2012;59:1-7.
Hahnel S, Rosentritt M, Handel G, Bürgers R In vitro
evaluation of artificial ageing on surface properties and early Candida albicans
adhesion to prosthetic resins. J Mater Sci Mater Med 2009;20:249-55.
[Figure 1], [Figure 2], [Figure 3], [Figure 4], [Figure 5]
[Table 1], [Table 2], [Table 3]